the $\phi$ values of (a) 0$^{\circ}$, (b) 30$^{\circ}$, (c) 90$^{\circ}$, (d) 180$^{\circ}$. Open symbols are the experimental data. Solid lines are the fit to the experimental data using Eq. (\[q7\]). Short dash and dotted lines are the symmetric ($V_{sym})$ and anti-symmetric ($V_{asym})$ components of the voltage](fig3.png){width="45.00000%"}

. \[fig3\]

The angle $\phi$ denotes the angle between measured voltage direction and the perpendicular direction of applied DC magnetic field (*H*). It has been previously found that CFMS thin films exhibit a cubic anisotropy \[33\].

   Sample   $V_{sp}$(V)$\times$$10^{-6}$   $V_{AHE}$(V)$\times$$10^{-6}$   $V_{AMR}^{\perp}$(V)$\times$$10^{-6}$   $V_{AMR}^{||}$(V)$\times$$10^{-6}$
  -------- ------------------------------ ------------------------------- --------------------------------------- ------------------------------------
     S1           3.93 $\pm$ 0.05                -1.14 $\pm$ 0.03                     2.97 $\pm$ 0.06                       0.16 $\pm$ 0.03
     S2           5.41 $\pm$ 0.16                -1.28 $\pm$ 0.04                     3.14 $\pm$ 0.18                       0.14 $\pm$ 0.04
     S3           2.88 $\pm$ 0.06                -0.78 $\pm$ 0.02                     1.54 $\pm$ 0.07                       0.09 $\pm$ 0.02
     S4           3.26 $\pm$ 0.05                -0.67 $\pm$ 0.05                     2.28 $\pm$ 0.06                       0.14 $\pm$ 0.03
     S5           0.89 $\pm$ 0.02                -0.64 $\pm$ 0.01                     0.67 $\pm$ 0.02                       0.05 $\pm$ 0.01

Angle dependent measurements of the voltage have been investigated to remove spin rectification effects e.g. anisotropic magnetoresistance (AMR), anomalous Hall effect (AHE). Fig. \[fig3\] shows the measured voltage (*$V_{meas}$*) (open blue symbol) versus *H* along with FMR signal (open black symbol) for sample 